data_1994-0358_4

_audit_update_record
;
2020-12-03 # Formatted by publCIF

;


 
_audit_creation_method            'SHELXL-2018/3'
_shelx_SHELXL_version_number      '2018/3'
_chemical_name_systematic         walstromite
_chemical_name_common             ?
_chemical_formula_moiety          ?
_chemical_formula_sum            'Ba1.14 Ca4 O18 Pb0.86 Si6' 
_chemical_formula_weight          951.61

loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'Ba'  'Ba'  -0.3244   2.2819
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Pb'  'Pb'  -3.3944  10.1111
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Ca'  'Ca'   0.2262   0.3064
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'O'  'O'   0.0106   0.0060
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Si'  'Si'   0.0817   0.0704
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_space_group_crystal_system       triclinic
_space_group_IT_number            2
_space_group_name_H-M_alt         'P -1'
_space_group_name_Hall            '-P 1'
 
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
 
loop_
 _space_group_symop_operation_xyz
 'x, y, z'
 '-x, -y, -z'
 
_cell_length_a                    6.73527(7)
_cell_length_b                    9.57172(12)
_cell_length_c                    6.68718(6)
_cell_angle_alpha                 110.1760(10)
_cell_angle_beta                  102.6060(10)
_cell_angle_gamma                 83.2060(10)
_cell_volume                      394.465(8)
_cell_formula_units_Z             1
_cell_measurement_temperature     293(2)
_cell_measurement_reflns_used     20080
_cell_measurement_theta_min       2.2670
_cell_measurement_theta_max       44.6520

_exptl_crystal_description        block
_exptl_crystal_colour             colourless
_exptl_crystal_density_diffrn     4.006          
_exptl_crystal_F_000              568
_exptl_crystal_size_max           0.199
_exptl_crystal_size_mid           0.151
_exptl_crystal_size_min           0.099
_exptl_absorpt_coefficient_mu     13.852
_shelx_estimated_absorpt_T_min    0.072
_shelx_estimated_absorpt_T_max    0.168
_exptl_absorpt_correction_type    multi-scan
_exptl_absorpt_correction_T_min   0.56824
_exptl_absorpt_correction_T_max   1.00000
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.40.62a (Rigaku Oxford Diffraction, 2019)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_diffrn_ambient_temperature       293(2)
_diffrn_radiation_wavelength      0.71073
_diffrn_radiation_type            MoK\a
_diffrn_source                    'micro-focus sealed X-ray tube'
_diffrn_source_type               'PhotonJet (Mo) X-ray Source'
_diffrn_radiation_probe           x-ray
_diffrn_radiation_monochromator   mirror
_diffrn_measurement_device        'four-circle diffractometer'
_diffrn_measurement_device_type   'XtaLAB Synergy,  HyPix'
_diffrn_detector                  'Hybrid Pixel Array Detector'
_diffrn_detector_type             HyPix
_diffrn_detector_area_resol_mean  10.0000
_diffrn_reflns_number             65908
_diffrn_reflns_av_unetI/netI      0.0295
_diffrn_reflns_av_R_equivalents   0.0572
_diffrn_reflns_limit_h_min        -13
_diffrn_reflns_limit_h_max        13
_diffrn_reflns_limit_k_min        -19
_diffrn_reflns_limit_k_max        19
_diffrn_reflns_limit_l_min        -13
_diffrn_reflns_limit_l_max        13
_diffrn_reflns_theta_min          2.269
_diffrn_reflns_theta_max          45.080
_diffrn_reflns_theta_full         25.242
_diffrn_measured_fraction_theta_max   0.999
_diffrn_measured_fraction_theta_full  1.000
_diffrn_reflns_Laue_measured_fraction_max    0.999
_diffrn_reflns_Laue_measured_fraction_full   1.000
_diffrn_reflns_point_group_measured_fraction_max   0.999
_diffrn_reflns_point_group_measured_fraction_full  1.000
_reflns_number_total              6531
_reflns_number_gt                 5677
_reflns_threshold_expression      'I > 2σ(I)'
_reflns_Friedel_coverage          0.000
_reflns_Friedel_fraction_max      .
_reflns_Friedel_fraction_full     .
 
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
 
_computing_data_collection     'CrysAlisPro 1.171.40.62a (Rigaku OD, 2019)'
_computing_cell_refinement     'CrysAlisPro 1.171.40.62a (Rigaku OD, 2019)'
_computing_data_reduction      'CrysAlisPro 1.171.40.62a (Rigaku OD, 2019)'
_computing_structure_refinement 'SHELXL-2018/3 (Sheldrick, 2018)'
_refine_special_details           ?
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0098P)²+3.7782P] where P=(Fo²+2Fc²)/3'
_refine_ls_extinction_method      'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_extinction_coef        0.0027(5)
_refine_ls_extinction_expression
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^'
_refine_ls_number_reflns          6531
_refine_ls_number_parameters      147
_refine_ls_number_restraints      0
_refine_ls_R_factor_all           0.0547
_refine_ls_R_factor_gt            0.0476
_refine_ls_wR_factor_ref          0.1047
_refine_ls_wR_factor_gt           0.1027
_refine_ls_goodness_of_fit_ref    1.250
_refine_ls_restrained_S_all       1.250
_refine_ls_shift/su_max           0.000
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_site_symmetry_order  
 _atom_site_calc_flag
 _atom_site_refinement_flags_posn
 _atom_site_refinement_flags_adp
 _atom_site_refinement_flags_occupancy
 _atom_site_disorder_assembly
 _atom_site_disorder_group
CA3A Ba 0.05053(16) 0.15010(8) 0.31843(17) 0.01179(13) Uani 0.570(4) 1 d . . P . .
CA3B Pb 0.08539(15) 0.16033(7) 0.28603(14) 0.01398(12) Uani 0.430(4) 1 d . . P . .
Ca1 Ca 0.27312(10) 0.49225(7) 0.76280(10) 0.01143(10) Uani 1 1 d . . . . .
Ca2 Ca 0.43927(9) 0.17017(7) 0.93833(10) 0.00998(10) Uani 1 1 d . . . . .
Si1 Si 0.09646(13) 0.77913(10) 0.15456(14) 0.00822(13) Uani 1 1 d . . . . .
Si2 Si 0.23322(14) 0.51723(10) 0.28343(14) 0.00817(13) Uani 1 1 d . . . . .
Si3 Si 0.44019(14) 0.80132(10) 0.51420(14) 0.00823(13) Uani 1 1 d . . . . .
O1 O 0.2317(4) 0.7409(3) 0.9718(4) 0.0115(4) Uani 1 1 d . . . . .
O2 O 0.1029(4) 0.1240(3) 0.9021(4) 0.0126(4) Uani 1 1 d . . . . .
O3 O 0.2328(4) 0.8750(3) 0.3927(4) 0.0107(3) Uani 1 1 d . . . . .
O4 O 0.0451(4) 0.6274(3) 0.1970(4) 0.0108(3) Uani 1 1 d . . . . .
O5 O 0.3734(4) 0.4423(3) 0.1066(4) 0.0107(3) Uani 1 1 d . . . . .
O6 O 0.1304(4) 0.4108(3) 0.3636(4) 0.0140(4) Uani 1 1 d . . . . .
O7 O 0.3600(4) 0.6405(3) 0.5057(4) 0.0115(4) Uani 1 1 d . . . . .
O8 O 0.4853(4) 0.0943(3) 0.2425(4) 0.0127(4) Uani 1 1 d . . . . .
O9 O 0.3856(4) 0.2369(3) 0.6289(4) 0.0111(3) Uani 1 1 d . . . . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
CA3A O6 2.516(3) . ?
CA3A O9 2.702(3) . ?
CA3A O2 2.726(3) 2_556 ?
CA3A O1 2.790(3) 2_566 ?
CA3A O2 2.805(3) 1_554 ?
CA3A O3 2.926(3) 1_545 ?
CA3A O8 3.035(3) . ?
CA3A O3 3.077(3) 2_566 ?
CA3A Si1 3.3330(11) 1_545 ?
CA3A Si1 3.3758(15) 2_565 ?
CA3A Si3 3.4025(14) 2_666 ?
CA3A Si3 3.6448(18) 2_566 ?
CA3B O6 2.314(3) . ?
CA3B O2 2.497(3) 1_554 ?
CA3B O9 2.655(2) . ?
CA3B O1 2.733(3) 2_566 ?
CA3B O8 2.748(3) . ?
CA3B Si1 3.1546(12) 2_565 ?
CA3B Si3 3.1946(13) 2_666 ?
CA3B Ca2 3.7040(16) 1_554 ?
CA3B Ca1 3.7498(8) . ?
CA3B Ca1 3.9371(8) 2_566 ?
Ca1 O1 2.327(3) . ?
Ca1 O9 2.387(3) . ?
Ca1 O5 2.427(3) 2_666 ?
Ca1 O5 2.444(2) 1_556 ?
Ca1 O6 2.506(3) . ?
Ca1 O4 2.650(2) 2_566 ?
Ca1 O7 2.762(3) . ?
Ca1 O6 2.811(3) 2_566 ?
Ca1 Si2 3.2470(11) . ?
Ca1 Si2 3.3657(11) 2_566 ?
Ca1 Si1 3.3830(11) 1_556 ?
Ca1 Si2 3.3937(11) 2_666 ?
Ca2 O2 2.305(3) . ?
Ca2 O9 2.313(3) . ?
Ca2 O8 2.334(3) 1_556 ?
Ca2 O1 2.347(3) 2_667 ?
Ca2 O8 2.446(3) 2_656 ?
Ca2 O5 2.484(3) 1_556 ?
Ca2 Si3 3.4038(11) 2_666 ?
Ca2 Si1 3.4372(11) 2_666 ?
Ca2 Si3 3.4932(11) 2_667 ?
Ca2 Si1 3.5294(11) 2_566 ?
Ca2 Ca2 3.5902(13) 2_657 ?
Si1 O2 1.591(3) 2_566 ?
Si1 O1 1.599(3) 1_554 ?
Si1 O4 1.660(3) . ?
Si1 O3 1.666(2) . ?
Si2 O6 1.585(3) . ?
Si2 O5 1.596(2) . ?
Si2 O7 1.675(3) . ?
Si2 O4 1.684(3) . ?
Si3 O8 1.593(3) 2_666 ?
Si3 O9 1.604(3) 2_666 ?
Si3 O3 1.666(3) . ?
Si3 O7 1.670(3) . ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
O6 CA3A O9 69.64(9) . . ?
O6 CA3A O2 155.35(9) . 2_556 ?
O9 CA3A O2 131.47(8) . 2_556 ?
O6 CA3A O1 69.89(9) . 2_566 ?
O9 CA3A O1 139.53(9) . 2_566 ?
O2 CA3A O1 87.91(8) 2_556 2_566 ?
O6 CA3A O2 77.41(9) . 1_554 ?
O9 CA3A O2 113.62(9) . 1_554 ?
O2 CA3A O2 81.29(9) 2_556 1_554 ?
O1 CA3A O2 55.78(7) 2_566 1_554 ?
O6 CA3A O3 142.71(9) . 1_545 ?
O9 CA3A O3 75.53(7) . 1_545 ?
O2 CA3A O3 55.96(7) 2_556 1_545 ?
O1 CA3A O3 142.96(7) 2_566 1_545 ?
O2 CA3A O3 105.67(8) 1_554 1_545 ?
O6 CA3A O8 80.36(9) . . ?
O9 CA3A O8 54.97(7) . . ?
O2 CA3A O8 101.31(7) 2_556 . ?
O1 CA3A O8 116.67(9) 2_566 . ?
O2 CA3A O8 63.99(8) 1_554 . ?
O3 CA3A O8 68.82(7) 1_545 . ?
O6 CA3A O3 115.71(8) . 2_566 ?
O9 CA3A O3 98.41(8) . 2_566 ?
O2 CA3A O3 77.45(8) 2_556 2_566 ?
O1 CA3A O3 99.49(7) 2_566 2_566 ?
O2 CA3A O3 147.97(7) 1_554 2_566 ?
O3 CA3A O3 81.74(8) 1_545 2_566 ?
O8 CA3A O3 143.81(7) . 2_566 ?
O6 CA3A Si1 157.30(9) . 1_545 ?
O9 CA3A Si1 104.06(6) . 1_545 ?
O2 CA3A Si1 28.24(5) 2_556 1_545 ?
O1 CA3A Si1 113.00(6) 2_566 1_545 ?
O2 CA3A Si1 85.96(6) 1_554 1_545 ?
O3 CA3A Si1 29.98(5) 1_545 1_545 ?
O8 CA3A Si1 78.48(5) . 1_545 ?
O3 CA3A Si1 86.49(6) 2_566 1_545 ?
O6 CA3A Si1 69.02(7) . 2_565 ?
O9 CA3A Si1 128.89(8) . 2_565 ?
O2 CA3A Si1 86.35(6) 2_556 2_565 ?
O1 CA3A Si1 28.05(5) 2_566 2_565 ?
O2 CA3A Si1 27.93(5) 1_554 2_565 ?
O3 CA3A Si1 128.87(6) 1_545 2_565 ?
O8 CA3A Si1 89.49(7) . 2_565 ?
O3 CA3A Si1 126.10(5) 2_566 2_565 ?
Si1 CA3A Si1 102.55(3) 1_545 2_565 ?
O6 CA3A Si3 69.38(7) . 2_666 ?
O9 CA3A Si3 27.54(5) . 2_666 ?
O2 CA3A Si3 122.11(6) 2_556 2_666 ?
O1 CA3A Si3 129.69(8) 2_566 2_666 ?
O2 CA3A Si3 87.38(7) 1_554 2_666 ?
O3 CA3A Si3 73.62(5) 1_545 2_666 ?
O8 CA3A Si3 27.91(5) . 2_666 ?
O3 CA3A Si3 124.27(5) 2_566 2_666 ?
Si1 CA3A Si3 94.80(3) 1_545 2_666 ?
Si1 CA3A Si3 107.98(5) 2_565 2_666 ?
O6 CA3A Si3 103.56(7) . 2_566 ?
O9 CA3A Si3 118.22(7) . 2_566 ?
O2 CA3A Si3 78.67(6) 2_556 2_566 ?
O1 CA3A Si3 72.51(6) 2_566 2_566 ?
O2 CA3A Si3 124.78(5) 1_554 2_566 ?
O3 CA3A Si3 104.30(7) 1_545 2_566 ?
O8 CA3A Si3 170.81(6) . 2_566 ?
O3 CA3A Si3 27.04(5) 2_566 2_566 ?
Si1 CA3A Si3 98.59(4) 1_545 2_566 ?
Si1 CA3A Si3 99.67(3) 2_565 2_566 ?
Si3 CA3A Si3 145.75(4) 2_666 2_566 ?
O6 CA3B O2 87.69(10) . 1_554 ?
O6 CA3B O9 73.45(9) . . ?
O2 CA3B O9 126.88(9) 1_554 . ?
O6 CA3B O1 73.79(9) . 2_566 ?
O2 CA3B O1 59.86(8) 1_554 2_566 ?
O9 CA3B O1 146.08(8) . 2_566 ?
O6 CA3B O8 90.36(10) . . ?
O2 CA3B O8 72.29(8) 1_554 . ?
O9 CA3B O8 59.06(7) . . ?
O1 CA3B O8 129.63(9) 2_566 . ?
O6 CA3B Si1 75.48(7) . 2_565 ?
O2 CA3B Si1 29.92(6) 1_554 2_565 ?
O9 CA3B Si1 141.73(8) . 2_565 ?
O1 CA3B Si1 30.45(5) 2_566 2_565 ?
O8 CA3B Si1 99.70(7) . 2_565 ?
O6 CA3B Si3 75.59(8) . 2_666 ?
O2 CA3B Si3 97.68(7) 1_554 2_666 ?
O9 CA3B Si3 30.07(5) . 2_666 ?
O1 CA3B Si3 142.32(7) 2_566 2_666 ?
O8 CA3B Si3 29.91(5) . 2_666 ?
Si1 CA3B Si3 119.44(5) 2_565 2_666 ?
O6 CA3B Ca2 75.05(8) . 1_554 ?
O2 CA3B Ca2 37.66(6) 1_554 1_554 ?
O9 CA3B Ca2 89.23(6) . 1_554 ?
O1 CA3B Ca2 90.70(6) 2_566 1_554 ?
O8 CA3B Ca2 39.00(6) . 1_554 ?
Si1 CA3B Ca2 61.32(3) 2_565 1_554 ?
Si3 CA3B Ca2 60.31(3) 2_666 1_554 ?
O6 CA3B Ca1 40.81(7) . . ?
O2 CA3B Ca1 124.68(7) 1_554 . ?
O9 CA3B Ca1 39.29(6) . . ?
O1 CA3B Ca1 107.29(6) 2_566 . ?
O8 CA3B Ca1 86.62(5) . . ?
Si1 CA3B Ca1 116.18(3) 2_565 . ?
Si3 CA3B Ca1 58.48(2) 2_666 . ?
Ca2 CA3B Ca1 97.29(3) 1_554 . ?
O6 CA3B Ca1 44.69(7) . 2_566 ?
O2 CA3B Ca1 83.55(6) 1_554 2_566 ?
O9 CA3B Ca1 111.34(6) . 2_566 ?
O1 CA3B Ca1 35.34(5) 2_566 2_566 ?
O8 CA3B Ca1 130.09(7) . 2_566 ?
Si1 CA3B Ca1 55.67(2) 2_565 2_566 ?
Si3 CA3B Ca1 120.26(3) 2_666 2_566 ?
Ca2 CA3B Ca1 98.48(3) 1_554 2_566 ?
Ca1 CA3B Ca1 72.123(18) . 2_566 ?
O6 CA3B CA3A 126.39(9) . 2 ?
O2 CA3B CA3A 40.45(7) 1_554 2 ?
O9 CA3B CA3A 141.24(6) . 2 ?
O1 CA3B CA3A 68.56(5) 2_566 2 ?
O8 CA3B CA3A 85.67(6) . 2 ?
Si1 CA3B CA3A 52.85(3) 2_565 2 ?
Si3 CA3B CA3A 115.42(5) 2_666 2 ?
Ca2 CA3B CA3A 68.83(4) 1_554 2 ?
Ca1 CA3B CA3A 165.01(7) . 2 ?
Ca1 CA3B CA3A 103.479(16) 2_566 2 ?
O1 Ca1 O9 164.73(9) . . ?
O1 Ca1 O5 79.74(8) . 2_666 ?
O9 Ca1 O5 88.93(9) . 2_666 ?
O1 Ca1 O5 86.27(9) . 1_556 ?
O9 Ca1 O5 80.87(8) . 1_556 ?
O5 Ca1 O5 74.80(9) 2_666 1_556 ?
O1 Ca1 O6 119.44(9) . . ?
O9 Ca1 O6 75.10(9) . . ?
O5 Ca1 O6 119.75(9) 2_666 . ?
O5 Ca1 O6 151.20(9) 1_556 . ?
O1 Ca1 O4 102.34(8) . 2_566 ?
O9 Ca1 O4 82.16(8) . 2_566 ?
O5 Ca1 O4 148.96(8) 2_666 2_566 ?
O5 Ca1 O4 74.45(8) 1_556 2_566 ?
O6 Ca1 O4 86.64(8) . 2_566 ?
O1 Ca1 O7 77.67(8) . . ?
O9 Ca1 O7 108.94(8) . . ?
O5 Ca1 O7 73.09(8) 2_666 . ?
O5 Ca1 O7 146.11(8) 1_556 . ?
O6 Ca1 O7 59.34(8) . . ?
O4 Ca1 O7 137.89(8) 2_566 . ?
O1 Ca1 O6 72.07(8) . 2_566 ?
O9 Ca1 O6 121.62(8) . 2_566 ?
O5 Ca1 O6 146.75(8) 2_666 2_566 ?
O5 Ca1 O6 119.48(8) 1_556 2_566 ?
O6 Ca1 O6 63.37(10) . 2_566 ?
O4 Ca1 O6 57.43(7) 2_566 2_566 ?
O7 Ca1 O6 83.79(8) . 2_566 ?
O1 Ca1 Si2 101.58(7) . . ?
O9 Ca1 Si2 89.78(6) . . ?
O5 Ca1 Si2 96.59(6) 2_666 . ?
O5 Ca1 Si2 167.30(6) 1_556 . ?
O6 Ca1 Si2 28.43(6) . . ?
O4 Ca1 Si2 112.96(6) 2_566 . ?
O7 Ca1 Si2 31.05(5) . . ?
O6 Ca1 Si2 72.79(6) 2_566 . ?
O1 Ca1 Si2 85.14(6) . 2_566 ?
O9 Ca1 Si2 104.49(6) . 2_566 ?
O5 Ca1 Si2 163.18(6) 2_666 2_566 ?
O5 Ca1 Si2 97.03(6) 1_556 2_566 ?
O6 Ca1 Si2 74.30(7) . 2_566 ?
O4 Ca1 Si2 29.58(5) 2_566 2_566 ?
O7 Ca1 Si2 110.89(6) . 2_566 ?
O6 Ca1 Si2 27.93(5) 2_566 2_566 ?
Si2 Ca1 Si2 93.60(3) . 2_566 ?
O1 Ca1 Si1 24.71(6) . 1_556 ?
O9 Ca1 Si1 149.77(7) . 1_556 ?
O5 Ca1 Si1 94.66(6) 2_666 1_556 ?
O5 Ca1 Si1 71.25(6) 1_556 1_556 ?
O6 Ca1 Si1 127.02(7) . 1_556 ?
O4 Ca1 Si1 79.40(6) 2_566 1_556 ?
O7 Ca1 Si1 100.79(6) . 1_556 ?
O6 Ca1 Si1 66.11(6) 2_566 1_556 ?
Si2 Ca1 Si1 119.45(3) . 1_556 ?
Si2 Ca1 Si1 68.63(3) 2_566 1_556 ?
O1 Ca1 Si2 100.00(7) . 2_666 ?
O9 Ca1 Si2 72.33(6) . 2_666 ?
O5 Ca1 Si2 25.56(6) 2_666 2_666 ?
O5 Ca1 Si2 91.51(6) 1_556 2_666 ?
O6 Ca1 Si2 96.02(7) . 2_666 ?
O4 Ca1 Si2 152.62(6) 2_566 2_666 ?
O7 Ca1 Si2 62.80(6) . 2_666 ?
O6 Ca1 Si2 146.57(6) 2_566 2_666 ?
Si2 Ca1 Si2 77.39(3) . 2_666 ?
Si2 Ca1 Si2 170.32(4) 2_566 2_666 ?
Si1 Ca1 Si2 118.79(3) 1_556 2_666 ?
O2 Ca2 O9 94.50(9) . . ?
O2 Ca2 O8 83.86(10) . 1_556 ?
O9 Ca2 O8 177.63(9) . 1_556 ?
O2 Ca2 O1 169.02(9) . 2_667 ?
O9 Ca2 O1 88.39(9) . 2_667 ?
O8 Ca2 O1 93.54(9) 1_556 2_667 ?
O2 Ca2 O8 90.54(9) . 2_656 ?
O9 Ca2 O8 95.66(9) . 2_656 ?
O8 Ca2 O8 82.66(9) 1_556 2_656 ?
O1 Ca2 O8 99.73(9) 2_667 2_656 ?
O2 Ca2 O5 91.72(9) . 1_556 ?
O9 Ca2 O5 81.49(9) . 1_556 ?
O8 Ca2 O5 100.24(9) 1_556 1_556 ?
O1 Ca2 O5 78.21(8) 2_667 1_556 ?
O8 Ca2 O5 176.49(9) 2_656 1_556 ?
O2 Ca2 Si3 114.35(7) . 2_666 ?
O9 Ca2 Si3 24.20(6) . 2_666 ?
O8 Ca2 Si3 156.12(7) 1_556 2_666 ?
O1 Ca2 Si3 71.35(6) 2_667 2_666 ?
O8 Ca2 Si3 81.89(6) 2_656 2_666 ?
O5 Ca2 Si3 94.74(6) 1_556 2_666 ?
O2 Ca2 Si1 164.64(7) . 2_666 ?
O9 Ca2 Si1 71.47(6) . 2_666 ?
O8 Ca2 Si1 109.96(7) 1_556 2_666 ?
O1 Ca2 Si1 23.75(6) 2_667 2_666 ?
O8 Ca2 Si1 84.83(7) 2_656 2_666 ?
O5 Ca2 Si1 92.30(6) 1_556 2_666 ?
Si3 Ca2 Si1 50.52(2) 2_666 2_666 ?
O2 Ca2 Si3 93.77(7) . 2_667 ?
O9 Ca2 Si3 160.17(7) . 2_667 ?
O8 Ca2 Si3 22.07(6) 1_556 2_667 ?
O1 Ca2 Si3 80.34(6) 2_667 2_667 ?
O8 Ca2 Si3 102.25(6) 2_656 2_667 ?
O5 Ca2 Si3 80.27(6) 1_556 2_667 ?
Si3 Ca2 Si3 151.66(4) 2_666 2_667 ?
Si1 Ca2 Si3 101.52(3) 2_666 2_667 ?
O2 Ca2 Si1 20.52(7) . 2_566 ?
O9 Ca2 Si1 80.04(6) . 2_566 ?
O8 Ca2 Si1 98.79(7) 1_556 2_566 ?
O1 Ca2 Si1 152.35(7) 2_667 2_566 ?
O8 Ca2 Si1 106.31(7) 2_656 2_566 ?
O5 Ca2 Si1 75.30(6) 1_556 2_566 ?
Si3 Ca2 Si1 102.96(3) 2_666 2_566 ?
Si1 Ca2 Si1 150.39(3) 2_666 2_566 ?
Si3 Ca2 Si1 102.66(3) 2_667 2_566 ?
O2 Ca2 Ca2 86.39(7) . 2_657 ?
O9 Ca2 Ca2 135.80(7) . 2_657 ?
O8 Ca2 Ca2 42.50(6) 1_556 2_657 ?
O1 Ca2 Ca2 98.93(7) 2_667 2_657 ?
O8 Ca2 Ca2 40.16(6) 2_656 2_657 ?
O5 Ca2 Ca2 142.71(6) 1_556 2_657 ?
Si3 Ca2 Ca2 119.89(3) 2_666 2_657 ?
Si1 Ca2 Ca2 99.24(3) 2_666 2_657 ?
Si3 Ca2 Ca2 62.74(2) 2_667 2_657 ?
Si1 Ca2 Ca2 106.90(3) 2_566 2_657 ?
O2 Ca2 Ca1 89.12(7) . . ?
O9 Ca2 Ca1 40.01(6) . . ?
O8 Ca2 Ca1 141.45(7) 1_556 . ?
O1 Ca2 Ca1 86.28(7) 2_667 . ?
O8 Ca2 Ca1 135.41(6) 2_656 . ?
O5 Ca2 Ca1 41.99(6) 1_556 . ?
Si3 Ca2 Ca1 58.12(2) 2_666 . ?
Si1 Ca2 Ca1 83.99(2) 2_666 . ?
Si3 Ca2 Ca1 122.26(3) 2_667 . ?
Si1 Ca2 Ca1 68.71(2) 2_566 . ?
Ca2 Ca2 Ca1 173.56(3) 2_657 . ?
O2 Si1 O1 110.27(14) 2_566 1_554 ?
O2 Si1 O4 112.78(14) 2_566 . ?
O1 Si1 O4 112.09(14) 1_554 . ?
O2 Si1 O3 109.33(14) 2_566 . ?
O1 Si1 O3 109.06(14) 1_554 . ?
O4 Si1 O3 103.02(13) . . ?
O2 Si1 CA3B 51.50(10) 2_566 2_565 ?
O1 Si1 CA3B 60.03(10) 1_554 2_565 ?
O4 Si1 CA3B 121.63(10) . 2_565 ?
O3 Si1 CA3B 135.14(10) . 2_565 ?
O2 Si1 CA3A 54.17(10) 2_566 1_565 ?
O1 Si1 CA3A 102.89(11) 1_554 1_565 ?
O4 Si1 CA3A 144.92(10) . 1_565 ?
O3 Si1 CA3A 61.35(9) . 1_565 ?
CA3B Si1 CA3A 78.17(3) 2_565 1_565 ?
O2 Si1 CA3A 55.65(10) 2_566 2_565 ?
O1 Si1 CA3A 55.17(10) 1_554 2_565 ?
O4 Si1 CA3A 125.13(10) . 2_565 ?
O3 Si1 CA3A 131.85(10) . 2_565 ?
CA3B Si1 CA3A 5.691(12) 2_565 2_565 ?
CA3A Si1 CA3A 77.45(3) 1_565 2_565 ?
O2 Si1 Ca1 121.04(10) 2_566 1_554 ?
O1 Si1 Ca1 37.48(10) 1_554 1_554 ?
O4 Si1 Ca1 75.29(9) . 1_554 ?
O3 Si1 Ca1 126.09(9) . 1_554 ?
CA3B Si1 Ca1 73.97(3) 2_565 1_554 ?
CA3A Si1 Ca1 139.74(4) 1_565 1_554 ?
CA3A Si1 Ca1 71.96(2) 2_565 1_554 ?
O2 Si1 Ca2 122.13(11) 2_566 2_666 ?
O1 Si1 Ca2 36.25(9) 1_554 2_666 ?
O4 Si1 Ca2 123.15(9) . 2_666 ?
O3 Si1 Ca2 72.86(9) . 2_666 ?
CA3B Si1 Ca2 85.30(3) 2_565 2_666 ?
CA3A Si1 Ca2 84.20(4) 1_565 2_666 ?
CA3A Si1 Ca2 79.62(3) 2_565 2_666 ?
Ca1 Si1 Ca2 65.25(2) 1_554 2_666 ?
O2 Si1 Ca2 30.50(10) 2_566 2_566 ?
O1 Si1 Ca2 124.68(10) 1_554 2_566 ?
O4 Si1 Ca2 82.29(9) . 2_566 ?
O3 Si1 Ca2 119.42(9) . 2_566 ?
CA3B Si1 Ca2 67.03(3) 2_565 2_566 ?
CA3A Si1 Ca2 80.09(3) 1_565 2_566 ?
CA3A Si1 Ca2 72.57(3) 2_565 2_566 ?
Ca1 Si1 Ca2 113.76(3) 1_554 2_566 ?
Ca2 Si1 Ca2 150.39(3) 2_666 2_566 ?
O2 Si1 CA3A 86.89(10) 2_566 2_566 ?
O1 Si1 CA3A 161.16(10) 1_554 2_566 ?
O4 Si1 CA3A 65.59(9) . 2_566 ?
O3 Si1 CA3A 55.90(9) . 2_566 ?
CA3B Si1 CA3A 138.12(4) 2_565 2_566 ?
CA3A Si1 CA3A 80.46(4) 1_565 2_566 ?
CA3A Si1 CA3A 142.54(4) 2_565 2_566 ?
Ca1 Si1 CA3A 138.84(3) 1_554 2_566 ?
Ca2 Si1 CA3A 127.71(3) 2_666 2_566 ?
Ca2 Si1 CA3A 74.10(2) 2_566 2_566 ?
O6 Si2 O5 117.93(15) . . ?
O6 Si2 O7 106.81(14) . . ?
O5 Si2 O7 111.40(14) . . ?
O6 Si2 O4 106.94(14) . . ?
O5 Si2 O4 111.04(13) . . ?
O7 Si2 O4 101.34(13) . . ?
O6 Si2 Ca1 48.84(10) . . ?
O5 Si2 Ca1 129.71(10) . . ?
O7 Si2 Ca1 58.28(9) . . ?
O4 Si2 Ca1 119.22(10) . . ?
O6 Si2 Ca1 56.19(11) . 2_566 ?
O5 Si2 Ca1 129.83(10) . 2_566 ?
O7 Si2 Ca1 117.79(10) . 2_566 ?
O4 Si2 Ca1 50.95(9) . 2_566 ?
Ca1 Si2 Ca1 86.40(3) . 2_566 ?
O6 Si2 Ca1 127.82(11) . 2_666 ?
O5 Si2 Ca1 41.02(9) . 2_666 ?
O7 Si2 Ca1 70.69(9) . 2_666 ?
O4 Si2 Ca1 124.94(9) . 2_666 ?
Ca1 Si2 Ca1 102.61(3) . 2_666 ?
Ca1 Si2 Ca1 170.32(4) 2_566 2_666 ?
O6 Si2 Ca1 130.27(11) . 1_554 ?
O5 Si2 Ca1 38.80(9) . 1_554 ?
O7 Si2 Ca1 122.34(10) . 1_554 ?
O4 Si2 Ca1 72.30(9) . 1_554 ?
Ca1 Si2 Ca1 168.47(4) . 1_554 ?
Ca1 Si2 Ca1 102.01(3) 2_566 1_554 ?
Ca1 Si2 Ca1 68.58(2) 2_666 1_554 ?
O8 Si3 O9 112.88(14) 2_666 2_666 ?
O8 Si3 O3 111.49(14) 2_666 . ?
O9 Si3 O3 110.01(13) 2_666 . ?
O8 Si3 O7 111.50(14) 2_666 . ?
O9 Si3 O7 107.83(14) 2_666 . ?
O3 Si3 O7 102.60(13) . . ?
O8 Si3 CA3B 59.34(10) 2_666 2_666 ?
O9 Si3 CA3B 56.02(9) 2_666 2_666 ?
O3 Si3 CA3B 144.48(10) . 2_666 ?
O7 Si3 CA3B 112.70(10) . 2_666 ?
O8 Si3 CA3A 63.10(10) 2_666 2_666 ?
O9 Si3 CA3A 51.14(9) 2_666 2_666 ?
O3 Si3 CA3A 140.21(10) . 2_666 ?
O7 Si3 CA3A 116.20(10) . 2_666 ?
CA3B Si3 CA3A 5.784(11) 2_666 2_666 ?
O8 Si3 Ca2 126.16(11) 2_666 2_666 ?
O9 Si3 Ca2 36.23(9) 2_666 2_666 ?
O3 Si3 Ca2 73.89(9) . 2_666 ?
O7 Si3 Ca2 119.51(9) . 2_666 ?
CA3B Si3 Ca2 85.14(3) 2_666 2_666 ?
CA3A Si3 Ca2 79.42(3) 2_666 2_666 ?
O8 Si3 Ca1 124.07(11) 2_666 2_666 ?
O9 Si3 Ca1 38.39(9) 2_666 2_666 ?
O3 Si3 Ca1 122.99(9) . 2_666 ?
O7 Si3 Ca1 69.71(9) . 2_666 ?
CA3B Si3 Ca1 68.89(2) 2_666 2_666 ?
CA3A Si3 Ca1 67.26(2) 2_666 2_666 ?
Ca2 Si3 Ca1 64.38(2) 2_666 2_666 ?
O8 Si3 Ca2 33.41(10) 2_666 2_667 ?
O9 Si3 Ca2 120.73(10) 2_666 2_667 ?
O3 Si3 Ca2 126.32(10) . 2_667 ?
O7 Si3 Ca2 78.54(9) . 2_667 ?
CA3B Si3 Ca2 67.09(3) 2_666 2_667 ?
CA3A Si3 Ca2 72.71(3) 2_666 2_667 ?
Ca2 Si3 Ca2 151.66(4) 2_666 2_667 ?
Ca1 Si3 Ca2 107.91(3) 2_666 2_667 ?
O8 Si3 CA3A 83.38(10) 2_666 2_566 ?
O9 Si3 CA3A 163.08(10) 2_666 2_566 ?
O3 Si3 CA3A 57.12(9) . 2_566 ?
O7 Si3 CA3A 68.09(9) . 2_566 ?
CA3B Si3 CA3A 140.90(4) 2_666 2_566 ?
CA3A Si3 CA3A 145.75(4) 2_666 2_566 ?
Ca2 Si3 CA3A 130.19(3) 2_666 2_566 ?
Ca1 Si3 CA3A 135.99(3) 2_666 2_566 ?
Ca2 Si3 CA3A 75.31(2) 2_667 2_566 ?
Si1 O1 Ca1 117.82(14) 1_556 . ?
Si1 O1 Ca2 120.00(13) 1_556 2_667 ?
Ca1 O1 Ca2 103.78(9) . 2_667 ?
Si1 O1 CA3B 89.52(11) 1_556 2_566 ?
Ca1 O1 CA3B 101.87(9) . 2_566 ?
Ca2 O1 CA3B 123.16(11) 2_667 2_566 ?
Si1 O1 CA3A 96.78(12) 1_556 2_566 ?
Ca1 O1 CA3A 101.39(9) . 2_566 ?
Ca2 O1 CA3A 115.97(10) 2_667 2_566 ?
CA3B O1 CA3A 8.058(13) 2_566 2_566 ?
Si1 O2 Ca2 128.98(15) 2_566 . ?
Si1 O2 CA3B 98.58(12) 2_566 1_556 ?
Ca2 O2 CA3B 100.89(10) . 1_556 ?
Si1 O2 CA3A 97.59(12) 2_566 2_556 ?
Ca2 O2 CA3A 122.63(10) . 2_556 ?
CA3B O2 CA3A 103.09(9) 1_556 2_556 ?
Si1 O2 CA3A 96.42(12) 2_566 1_556 ?
Ca2 O2 CA3A 105.88(10) . 1_556 ?
CA3B O2 CA3A 5.264(19) 1_556 1_556 ?
CA3A O2 CA3A 98.71(9) 2_556 1_556 ?
Si3 O3 Si1 122.39(15) . . ?
Si3 O3 CA3A 143.70(13) . 1_565 ?
Si1 O3 CA3A 88.67(10) . 1_565 ?
Si3 O3 CA3A 95.83(11) . 2_566 ?
Si1 O3 CA3A 97.47(11) . 2_566 ?
CA3A O3 CA3A 98.26(8) 1_565 2_566 ?
Si1 O4 Si2 121.01(15) . . ?
Si1 O4 Ca1 138.55(13) . 2_566 ?
Si2 O4 Ca1 99.47(11) . 2_566 ?
Si2 O5 Ca1 113.42(13) . 2_666 ?
Si2 O5 Ca1 117.06(13) . 1_554 ?
Ca1 O5 Ca1 105.20(9) 2_666 1_554 ?
Si2 O5 Ca2 125.38(13) . 1_554 ?
Ca1 O5 Ca2 96.97(9) 2_666 1_554 ?
Ca1 O5 Ca2 95.18(8) 1_554 1_554 ?
Si2 O6 CA3B 140.41(16) . . ?
Si2 O6 Ca1 102.74(13) . . ?
CA3B O6 Ca1 102.08(10) . . ?
Si2 O6 CA3A 148.35(16) . . ?
CA3B O6 CA3A 7.981(18) . . ?
Ca1 O6 CA3A 97.72(9) . . ?
Si2 O6 Ca1 95.89(13) . 2_566 ?
CA3B O6 Ca1 99.94(10) . 2_566 ?
Ca1 O6 Ca1 116.63(10) . 2_566 ?
CA3A O6 Ca1 96.21(9) . 2_566 ?
Si3 O7 Si2 124.77(15) . . ?
Si3 O7 Ca1 142.93(13) . . ?
Si2 O7 Ca1 90.67(11) . . ?
Si3 O8 Ca2 124.52(14) 2_666 1_554 ?
Si3 O8 Ca2 130.73(15) 2_666 2_656 ?
Ca2 O8 Ca2 97.34(9) 1_554 2_656 ?
Si3 O8 CA3B 90.75(12) 2_666 . ?
Ca2 O8 CA3B 93.20(9) 1_554 . ?
Ca2 O8 CA3B 113.69(10) 2_656 . ?
Si3 O8 CA3A 88.98(11) 2_666 . ?
Ca2 O8 CA3A 98.33(9) 1_554 . ?
Ca2 O8 CA3A 111.39(9) 2_656 . ?
CA3B O8 CA3A 5.314(17) . . ?
Si3 O9 Ca2 119.56(13) 2_666 . ?
Si3 O9 Ca1 116.94(14) 2_666 . ?
Ca2 O9 Ca1 101.45(9) . . ?
Si3 O9 CA3B 93.91(11) 2_666 . ?
Ca2 O9 CA3B 127.92(11) . . ?
Ca1 O9 CA3B 95.94(8) . . ?
Si3 O9 CA3A 101.32(12) 2_666 . ?
Ca2 O9 CA3A 120.04(11) . . ?
Ca1 O9 CA3A 95.81(8) . . ?
CA3B O9 CA3A 8.339(13) . . ?
 
loop_
 _geom_torsion_atom_site_label_1
 _geom_torsion_atom_site_label_2
 _geom_torsion_atom_site_label_3
 _geom_torsion_atom_site_label_4
 _geom_torsion
 _geom_torsion_site_symmetry_1
 _geom_torsion_site_symmetry_2
 _geom_torsion_site_symmetry_3
 _geom_torsion_site_symmetry_4
 _geom_torsion_publ_flag
O8 Si3 O3 Si1 -168.99(17) 2_666 . . . ?
O9 Si3 O3 Si1 65.0(2) 2_666 . . . ?
O7 Si3 O3 Si1 -49.5(2) . . . . ?
CA3B Si3 O3 Si1 124.08(15) 2_666 . . . ?
CA3A Si3 O3 Si1 117.69(16) 2_666 . . . ?
Ca2 Si3 O3 Si1 67.90(16) 2_666 . . . ?
Ca1 Si3 O3 Si1 24.3(2) 2_666 . . . ?
Ca2 Si3 O3 Si1 -134.48(13) 2_667 . . . ?
CA3A Si3 O3 Si1 -102.68(18) 2_566 . . . ?
O8 Si3 O3 CA3A 46.2(3) 2_666 . . 1_565 ?
O9 Si3 O3 CA3A -79.8(2) 2_666 . . 1_565 ?
O7 Si3 O3 CA3A 165.7(2) . . . 1_565 ?
CA3B Si3 O3 CA3A -20.7(3) 2_666 . . 1_565 ?
CA3A Si3 O3 CA3A -27.1(3) 2_666 . . 1_565 ?
Ca2 Si3 O3 CA3A -76.9(2) 2_666 . . 1_565 ?
Ca1 Si3 O3 CA3A -120.51(19) 2_666 . . 1_565 ?
Ca2 Si3 O3 CA3A 80.7(2) 2_667 . . 1_565 ?
CA3A Si3 O3 CA3A 112.5(2) 2_566 . . 1_565 ?
O8 Si3 O3 CA3A -66.31(14) 2_666 . . 2_566 ?
O9 Si3 O3 CA3A 167.68(11) 2_666 . . 2_566 ?
O7 Si3 O3 CA3A 53.14(12) . . . 2_566 ?
CA3B Si3 O3 CA3A -133.23(12) 2_666 . . 2_566 ?
CA3A Si3 O3 CA3A -139.63(10) 2_666 . . 2_566 ?
Ca2 Si3 O3 CA3A 170.58(8) 2_666 . . 2_566 ?
Ca1 Si3 O3 CA3A 126.97(6) 2_666 . . 2_566 ?
Ca2 Si3 O3 CA3A -31.79(12) 2_667 . . 2_566 ?
O2 Si1 O3 Si3 173.92(17) 2_566 . . . ?
O1 Si1 O3 Si3 -65.4(2) 1_554 . . . ?
O4 Si1 O3 Si3 53.8(2) . . . . ?
CA3B Si1 O3 Si3 -131.73(13) 2_565 . . . ?
CA3A Si1 O3 Si3 -160.0(2) 1_565 . . . ?
CA3A Si1 O3 Si3 -125.32(14) 2_565 . . . ?
Ca1 Si1 O3 Si3 -27.4(2) 1_554 . . . ?
Ca2 Si1 O3 Si3 -67.29(16) 2_666 . . . ?
Ca2 Si1 O3 Si3 142.19(13) 2_566 . . . ?
CA3A Si1 O3 Si3 101.80(18) 2_566 . . . ?
O2 Si1 O3 CA3A -26.04(14) 2_566 . . 1_565 ?
O1 Si1 O3 CA3A 94.60(12) 1_554 . . 1_565 ?
O4 Si1 O3 CA3A -146.18(10) . . . 1_565 ?
CA3B Si1 O3 CA3A 28.31(15) 2_565 . . 1_565 ?
CA3A Si1 O3 CA3A 34.72(14) 2_565 . . 1_565 ?
Ca1 Si1 O3 CA3A 132.67(7) 1_554 . . 1_565 ?
Ca2 Si1 O3 CA3A 92.75(7) 2_666 . . 1_565 ?
Ca2 Si1 O3 CA3A -57.77(10) 2_566 . . 1_565 ?
CA3A Si1 O3 CA3A -98.16(9) 2_566 . . 1_565 ?
O2 Si1 O3 CA3A 72.12(13) 2_566 . . 2_566 ?
O1 Si1 O3 CA3A -167.25(11) 1_554 . . 2_566 ?
O4 Si1 O3 CA3A -48.03(12) . . . 2_566 ?
CA3B Si1 O3 CA3A 126.47(9) 2_565 . . 2_566 ?
CA3A Si1 O3 CA3A 98.16(9) 1_565 . . 2_566 ?
CA3A Si1 O3 CA3A 132.87(8) 2_565 . . 2_566 ?
Ca1 Si1 O3 CA3A -129.17(7) 1_554 . . 2_566 ?
Ca2 Si1 O3 CA3A -169.09(8) 2_666 . . 2_566 ?
Ca2 Si1 O3 CA3A 40.38(10) 2_566 . . 2_566 ?
O2 Si1 O4 Si2 -173.89(16) 2_566 . . . ?
O1 Si1 O4 Si2 61.0(2) 1_554 . . . ?
O3 Si1 O4 Si2 -56.1(2) . . . . ?
CA3B Si1 O4 Si2 128.41(14) 2_565 . . . ?
CA3A Si1 O4 Si2 -114.33(16) 1_565 . . . ?
CA3A Si1 O4 Si2 123.04(14) 2_565 . . . ?
Ca1 Si1 O4 Si2 68.21(15) 1_554 . . . ?
Ca2 Si1 O4 Si2 21.7(2) 2_666 . . . ?
Ca2 Si1 O4 Si2 -174.67(17) 2_566 . . . ?
CA3A Si1 O4 Si2 -98.68(17) 2_566 . . . ?
O2 Si1 O4 Ca1 -7.9(3) 2_566 . . 2_566 ?
O1 Si1 O4 Ca1 -133.03(19) 1_554 . . 2_566 ?
O3 Si1 O4 Ca1 109.9(2) . . . 2_566 ?
CA3B Si1 O4 Ca1 -65.6(2) 2_565 . . 2_566 ?
CA3A Si1 O4 Ca1 51.7(3) 1_565 . . 2_566 ?
CA3A Si1 O4 Ca1 -70.9(2) 2_565 . . 2_566 ?
Ca1 Si1 O4 Ca1 -125.8(2) 1_554 . . 2_566 ?
Ca2 Si1 O4 Ca1 -172.27(13) 2_666 . . 2_566 ?
Ca2 Si1 O4 Ca1 -8.65(18) 2_566 . . 2_566 ?
CA3A Si1 O4 Ca1 67.34(17) 2_566 . . 2_566 ?
O6 Si2 O4 Si1 165.62(17) . . . . ?
O5 Si2 O4 Si1 -64.5(2) . . . . ?
O7 Si2 O4 Si1 53.9(2) . . . . ?
Ca1 Si2 O4 Si1 113.79(15) . . . . ?
Ca1 Si2 O4 Si1 170.7(2) 2_566 . . . ?
Ca1 Si2 O4 Si1 -20.3(2) 2_666 . . . ?
Ca1 Si2 O4 Si1 -66.64(15) 1_554 . . . ?
O6 Si2 O4 Ca1 -5.05(15) . . . 2_566 ?
O5 Si2 O4 Ca1 124.86(12) . . . 2_566 ?
O7 Si2 O4 Ca1 -116.73(12) . . . 2_566 ?
Ca1 Si2 O4 Ca1 -56.88(11) . . . 2_566 ?
Ca1 Si2 O4 Ca1 169.02(5) 2_666 . . 2_566 ?
Ca1 Si2 O4 Ca1 122.69(9) 1_554 . . 2_566 ?
O6 Si2 O5 Ca1 -116.62(16) . . . 2_666 ?
O7 Si2 O5 Ca1 7.38(18) . . . 2_666 ?
O4 Si2 O5 Ca1 119.52(13) . . . 2_666 ?
Ca1 Si2 O5 Ca1 -58.50(17) . . . 2_666 ?
Ca1 Si2 O5 Ca1 175.59(5) 2_566 . . 2_666 ?
Ca1 Si2 O5 Ca1 122.83(19) 1_554 . . 2_666 ?
O6 Si2 O5 Ca1 120.55(16) . . . 1_554 ?
O7 Si2 O5 Ca1 -115.45(14) . . . 1_554 ?
O4 Si2 O5 Ca1 -3.31(18) . . . 1_554 ?
Ca1 Si2 O5 Ca1 178.67(6) . . . 1_554 ?
Ca1 Si2 O5 Ca1 52.76(18) 2_566 . . 1_554 ?
Ca1 Si2 O5 Ca1 -122.83(19) 2_666 . . 1_554 ?
O6 Si2 O5 Ca2 1.4(2) . . . 1_554 ?
O7 Si2 O5 Ca2 125.40(15) . . . 1_554 ?
O4 Si2 O5 Ca2 -122.46(15) . . . 1_554 ?
Ca1 Si2 O5 Ca2 59.52(19) . . . 1_554 ?
Ca1 Si2 O5 Ca2 -66.39(19) 2_566 . . 1_554 ?
Ca1 Si2 O5 Ca2 118.0(2) 2_666 . . 1_554 ?
Ca1 Si2 O5 Ca2 -119.2(2) 1_554 . . 1_554 ?
O5 Si2 O6 CA3B -7.8(3) . . . . ?
O7 Si2 O6 CA3B -134.0(2) . . . . ?
O4 Si2 O6 CA3B 118.1(2) . . . . ?
Ca1 Si2 O6 CA3B -127.6(3) . . . . ?
Ca1 Si2 O6 CA3B 113.4(3) 2_566 . . . ?
Ca1 Si2 O6 CA3B -55.7(3) 2_666 . . . ?
Ca1 Si2 O6 CA3B 37.2(3) 1_554 . . . ?
O5 Si2 O6 Ca1 119.81(14) . . . . ?
O7 Si2 O6 Ca1 -6.45(16) . . . . ?
O4 Si2 O6 Ca1 -114.30(13) . . . . ?
Ca1 Si2 O6 Ca1 -119.03(14) 2_566 . . . ?
Ca1 Si2 O6 Ca1 71.85(14) 2_666 . . . ?
Ca1 Si2 O6 Ca1 164.82(5) 1_554 . . . ?
O5 Si2 O6 CA3A -9.2(4) . . . . ?
O7 Si2 O6 CA3A -135.4(3) . . . . ?
O4 Si2 O6 CA3A 116.7(3) . . . . ?
Ca1 Si2 O6 CA3A -129.0(4) . . . . ?
Ca1 Si2 O6 CA3A 112.0(3) 2_566 . . . ?
Ca1 Si2 O6 CA3A -57.1(3) 2_666 . . . ?
Ca1 Si2 O6 CA3A 35.8(4) 1_554 . . . ?
O5 Si2 O6 Ca1 -121.16(13) . . . 2_566 ?
O7 Si2 O6 Ca1 112.58(12) . . . 2_566 ?
O4 Si2 O6 Ca1 4.72(14) . . . 2_566 ?
Ca1 Si2 O6 Ca1 119.03(14) . . . 2_566 ?
Ca1 Si2 O6 Ca1 -169.13(5) 2_666 . . 2_566 ?
Ca1 Si2 O6 Ca1 -76.16(13) 1_554 . . 2_566 ?
O8 Si3 O7 Si2 168.50(18) 2_666 . . . ?
O9 Si3 O7 Si2 -67.1(2) 2_666 . . . ?
O3 Si3 O7 Si2 49.1(2) . . . . ?
CA3B Si3 O7 Si2 -126.93(16) 2_666 . . . ?
CA3A Si3 O7 Si2 -121.87(16) 2_666 . . . ?
Ca2 Si3 O7 Si2 -29.4(2) 2_666 . . . ?
Ca1 Si3 O7 Si2 -71.75(17) 2_666 . . . ?
Ca2 Si3 O7 Si2 174.09(19) 2_667 . . . ?
CA3A Si3 O7 Si2 95.47(18) 2_566 . . . ?
O8 Si3 O7 Ca1 8.0(3) 2_666 . . . ?
O9 Si3 O7 Ca1 132.5(2) 2_666 . . . ?
O3 Si3 O7 Ca1 -111.4(2) . . . . ?
CA3B Si3 O7 Ca1 72.6(2) 2_666 . . . ?
CA3A Si3 O7 Ca1 77.7(2) 2_666 . . . ?
Ca2 Si3 O7 Ca1 170.13(16) 2_666 . . . ?
Ca1 Si3 O7 Ca1 127.8(2) 2_666 . . . ?
Ca2 Si3 O7 Ca1 13.61(19) 2_667 . . . ?
CA3A Si3 O7 Ca1 -65.0(2) 2_566 . . . ?
O6 Si2 O7 Si3 -162.67(19) . . . . ?
O5 Si2 O7 Si3 67.3(2) . . . . ?
O4 Si2 O7 Si3 -50.9(2) . . . . ?
Ca1 Si2 O7 Si3 -168.4(2) . . . . ?
Ca1 Si2 O7 Si3 -102.54(17) 2_566 . . . ?
Ca1 Si2 O7 Si3 72.38(17) 2_666 . . . ?
Ca1 Si2 O7 Si3 25.2(2) 1_554 . . . ?
O6 Si2 O7 Ca1 5.70(14) . . . . ?
O5 Si2 O7 Ca1 -124.37(12) . . . . ?
O4 Si2 O7 Ca1 117.48(11) . . . . ?
Ca1 Si2 O7 Ca1 65.84(9) 2_566 . . . ?
Ca1 Si2 O7 Ca1 -119.25(7) 2_666 . . . ?
Ca1 Si2 O7 Ca1 -166.41(5) 1_554 . . . ?
 
_refine_diff_density_max    3.379
_refine_diff_density_min   -1.840
_refine_diff_density_rms    0.283


loop_
_publcif_info_cif.paper_type
 ?



_publcif_funding_html
;
;
